Preparation of PMMA/hBN Composite Coatings for · PDF filePreparation of PMMA/hBN Composite...
Embed Size (px)
Transcript of Preparation of PMMA/hBN Composite Coatings for · PDF filePreparation of PMMA/hBN Composite...
*e-mail: [email protected]
Preparation of PMMA/hBN Composite Coatings for Metal Surface Protection
T. Coana*, G. S. Barrosob, G. Motzb, A. Bolzna, R. A. F. Machadoa
aDepartamento de Engenharia Qumica e Engenharia de Alimentos, Federal University of Santa Catarina UFSC, Campus Universitrio, Trindade, CP 476, CEP 88010-970, Florianpolis, SC, Brazil
bUniversity of Bayreuth, Bayreuth, Germany - Lehrstuhl Keramische Werkstoffe, Ludwig-Thoma-Str. 36b, 95447, Bayreuth, Bayern, Germany
Received: February 5, 2013; Revised: June 10, 2013
Polyacrylics have been widely used in coatings. However, their application is limited by low corrosion resistance. One way to enhance their properties is the addition of fillers with adequate properties. In this study, composite materials of PMMA and hBN were developed and deposited on steel by dip-coating. The influence of the amount of hBN in the PMMA coating regarding corrosion resistance was investigated. The surface and cross-section of the coatings were characterized by SEM, the porosity was investigated by systematic manual point count and the adhesion was classified according to the tape test standard. The produced coatings were submersed in NaCl and HCl solutions to analyze corrosion resistance. The results showed that the PMMA/hBN composite coatings improved the corrosion resistance in comparison with pure PMMA. Additionally, the coatings are crack free and well bonded to the metallic substrate.
Keywords: Poly(methyl methacrylate), boron nitride, composite coatings, corrosion resistance, dip-coating
1. IntroductionPolyacrylics have increasingly been used as coatings,
paints and adhesives due to their excellent performance of film-forming and good cohesiveness1,2, good weatherability, high strength, and excellent dimensional stability3. However, the low corrosion resistance limits their applications.
In order to improve corrosion resistance, the most commonly used strategy to reduce the release of ions is through surface modification methods, including surface passivation, electrochemical polishing, and polymer-derived ceramic coatings4-6. However, for less aggressive environments, the application of such methods is not economically interesting. Therefore, the fabrication of polymeric coatings with protective performance and lower cost is an important technological improvement.
A suitable way to enhance the properties of the polymeric coatings is the addition of specific filler materials with the desired characteristic7. Boron nitride (BN) is a material widely used in technological applications due to its unique chemical and physical properties, such as low density, high melting point, high thermal conductivity, good chemical resistance and inertness, low friction coefficient, high oxidation resistance, significantly high wear resistance and high electrical resistivity8,9. This ceramic is applied in bulk form and as thin films, fibers and coatings in electronic and ceramic composite applications10. BN has at least five known crystalline forms: cubic (cBN), hexagonal (hBN), wurtzite (wBN), rhombohedral (rBN) and rocksalt structure11,12. For coating purposes, the lamellar structure of the hexagonal phase is the most interesting3, as it enables the
particles to align with the surface during coating application, improving the barrier properties13.
In this study, the method chosen to apply the coatings on the metal substrates is the dip-coating, which is an extensively used lacquer method. It stands out among available polymer coating methods like pulsed laser deposition (PLD)14 or thermal spraying15 due to its simplicity and low cost. In comparison with other simple and traditional polymer coating methods like spin-coating and spray-coating, dip-coating is more suitable for geometries like sheets, pipes and fibers, due to easy reproducibility of experimental conditions. In this processing, the solid substrates are simply immersed into a coating slurry, and withdrawn with controlled hoisting speed14-17. The main parameters in this coating process are the viscosity and density of the coating mixture, and the hoisting speed, which together determine the coating thickness18.
Zhi et al.19 manufactured composites of polystyrene and BN nanotubes (PS/BNNT) using a simple sonication-assisted solution-evaporation method. The tensile tests revealed that the elastic modulus increased up to 21% with just 1 wt. (%) BNNT fraction. Furthermore, the composites showed a better resistance to oxidation than the pure polymer.
Zhi et al.20 fabricated poly(methyl methacrylate) and BNNT (PMMA/BNNT) composites and investigated their mechanical and thermal properties. The elastic modulus of PMMA was improved up to 19% using only a 1 wt. (%) BNNT loading fraction. The PMMA/BNNT composite films simultaneously possessing (i) improved thermal conductivity, (ii) enhanced mechanical properties and
Materials Research. 2013; 16(6): 1366-1372 2013DI:D 10.1590/S1516-14392013005000140
Preparation of PMMA/hBN Composite Coatings for Metal Surface Protection
(iii) perfect electrical insulation are expected to attend several applications in many polymeric fields.
Kiran et al.21 prepared PMMA/BN composites (containing 3 wt. (%) of BN) and studied the dependence of the mechanical properties on the number of BN particle layers. Experimental results showed that the hardness and elastic modulus of the PMMA/BN composite were higher in comparison with pure PMMA. Additionally, as the number of BN particle layers decreases, the effective surface area increases, enabling greater interactions between BN and PMMA. The authors concluded that this is the reason why the composite with the least number of BN layers has the highest stiffness and hardness.
Song et al.22 exfoliated hexagonal BN in organic medium and dispersed the resulting BN nanosheets in poly(vinyl alcohol) (PVA) and epoxy matrices. The results suggested that nanometric BN sheets provide films with superior thermal conductivity.
Madakbas et al.23 fabricated polyacrylonitrile (PAN)/hBN composite coatings to investigate flame retardancy and thermal stability. The results showed that the limiting oxygen index (LDI) value of the composites increased up to 27% with the addition of hBN. The glass transition temperature (Tg) of PAN was found to be 83 C, and with 10% hBN the Tg raised to 112 C. The authors attributed this behavior to the loss of mobility of the polymer chains due to the decrease in the free volume of the composites.
Although some studies in the field of PMMA/BN composites have been conducted, surprisingly the influence of the amount of BN in the PMMA coating regarding corrosion resistance has been neglected so far.
In the present study, composite materials of PMMA and hBN powder were developed, and the influence of the amount of hBN in the PMMA coating regarding corrosion resistance was evaluated. The composite coatings were deposited on AISI 304 stainless steel substrates. The surface and cross-section of the coatings were characterized by Scanning Electron Microscopy (SEM), the porosity was investigated by systematic manual point count (ASTM E 562-02)24 and the adhesion was investigated by tape test standard (ASTM D 3359)25. Additionally, the produced coatings were submersed in aqueous NaCl and HCl solutions to analyze corrosion resistance.
The monomer methyl methacrylate (MMA), the initiator dicumyl peroxide (DCP) and the solvent toluene, were acquired from Sigma-Aldrich Corporation. Hexagonal boron nitride, used as passive filler, with a particle size D50 = 0.7 m was obtained from Henze BNP GmbH. Disperbyk 2070, from BYK-Chemie GmbH, was used as an additive to disperse the ceramic powder. All the reagents were used as received, without further purification.
2.2. Synthesis of PMMA
Solution polymerization reactions were carried out in batch at 130 C for 4 hours under pressure. In a typical
procedure, 50.00 g toluene, 5.00 g MMA and 0.405 g DCP were added to 100-ml stainless steel reactor equipped with a thermometer, argon inlet, and mechanical stirrer. After the polymerization reaction, toluene and residual monomer were removed from the mixture under reduced pressure for 4 hours. The average molecular weight of the purified PMMA, measured by gel permeation chromatography (GPC), is Mw = 320 000 g/mol (Mw/Mn = 1.42).
2.3. Preparation of PMMA/BN composite coatings
The hBN powder and the dispersant agent were added to toluene and treated in an ultrasound bath at 50 C for 15 minutes, followed by a vigorous mechanical stirring for 24 hours. The formed stable suspension was used in subsequent procedures. The synthesized PMMA was dissolved in toluene under mechanical stirring for 5 hours, forming a 15 wt. (%) solution. This solution was then mixed with different volumes of the hBN suspension. The sample codes and the resulting coating compositions after drying are given in Table 1.
2.4. Substrate preparation and film depositionThe AISI 304 stainless steel substrates were cut into
60 30 mm sheets, sandblasted, cleaned in ultrasound bath with acetone and dried at room temperature. The dip-coating method (RDC 15 Relamatic, Glattburg, Switzerland) was used to apply the coatings to the steel sheets. In this procedure, the substrates were immersed in the coating slurry for 10 seconds and withdrawn with hoisting speed of 0.3 m/min (Figure 1). Finally, the coated AISI 304 substrates were dried at 110 C in air for 12 hours.
Table 1. Specification of PMMA/hBN composite coatings.
PMMA wt. (%) hBN wt. (%)
A 100 0B 90 10C 70 30D 50 50E 30 70
Figure 1. Schematic representation of dip-coating process.
2013; 16(6) 1367
Coan et al.